Successfully reported this slideshow.
You’ve unlocked unlimited downloads on SlideShare!
Metals Bioaccumulation Mechanism in Neem Bark
Kishore K. Krishnani1 • Veera M. Boddu2 • Deok Hyun Moon3 • S. V. Ghadge1 •
Biplab Sarkar1 • M. P. Brahmane1 • K. Choudhary4 • V. Kathiravan5 •
Received: 18 October 2014 / Accepted: 15 July 2015
Ó Springer Science+Business Media New York 2015
Abstract The aim of this work was to deﬁne the bioac-
cumulation mechanism of metals onto the non-living bio-
material prepared from an extensively available plant bark
biomass of neem (Azadirachta indica). Based on maximum
ultimate ﬁxation capacities (mmol/g) of the product, metals
ions could be arranged as Hg2?
Surface properties of the biomaterial were characterized by
X-ray photoelectron spectroscopy and X-ray diffraction
techniques for their sorption mechanism. Whewellite
(C2CaO4ÁH2O) was identiﬁed in the biomaterial, which
indicated that calcium ions are electrovalently bonded
with carboxylate ions facilitating the ion exchange
mechanism with metal ions. Bioaccumulation of metal
ions was also studied by Fourier transform infrared
spectroscopy, which indicated the presence of functional
groups implicated in adsorbing metal ions. Biomaterial
did not adsorb anionic As(III), As(V) and Cr(VI), because
of their electrostatic repulsion with carboxylic functional
groups. Neem bark can be used as bioindicators, bioac-
cumulators and biomonitors while determining environ-
mental pressures. Metal bioaccumulative properties and
structural investigation of plant bark has potential in
providing quantitative information on the metal contam-
ination in the surrounding environment.
Keywords Biomaterial Á Characterization Á Toxicants Á
Removal Á Whewellite Á Ion exchange
During recent years, interests have been primarily focused
on metals due to their known toxicity, as they are dis-
charged in small quantities into the environment by
numerous activities. Human food chain effects have been
of great concern, because of an increasing metal accumu-
lation and their potential adverse health impact. For these
reasons, legislations governing levels of contaminants are
becoming more stringent. Unlike organic compounds,
metals are non-biodegradable and tend to accumulate in
plants (Bulut and Baysal 2006; Krishnani and Ayyappan
2006), which can be used as bioindicators, bioaccumulators
and biomonitors while determining environmental pres-
sures (Samecka-Cymerman et al. 2006). In biosorption,
complexes are formed between metal ions and the ligands
or functional groups of biological material. Mechanisms of
metal uptake are not always known, especially in the plant
barks, which are metal bioaccumulator. The examination of
the functional groups is crucial in bioaccumulation of
metals in the native or modiﬁed bark materials, but little
attention has been paid to the identiﬁcation of the active
binding sites and cations involved in metal uptake (Gloa-
guen and Morvan 1997; Athar et al. 2007; Arshad et al.
2008; Maharia et al. 2010). In the present investigation,
new biomaterial prepared from plant bark of neem (Aza-
dirachta indica) has been evaluated for its bioaccumulation
mechanism of Hg, Cd, Pb, Cu, As and Cr with respect to
individual and multi component systems.
& Kishore K. Krishnani
National Institute of Abiotic Stress Management,
Baramati, Pune 413115, India
US Army Construction Engineering Research Laboratories,
Champaign, IL, USA
Department of Environmental Engineering, Chosun
University, Gwangju 501759, Korea
Directorate of Weed Science Research, Jabalpur, India
The Madura College, Madurai, TN, India
CEE, Stevens Institute of Technology, Hoboken, NJ 07030,
Bull Environ Contam Toxicol
Materials and Methods
Metal stock solutions (10,000 mg/L) were prepared by
dissolving appropriate amount (1 g) of metal salt [CuCl2Á
2H2O, HgCl2, CdCl2Á2.5H2O, Pb(NO3)2, K2Cr2O7, NaAsO2,
NaH2AsO4] in 100 mL of deionized water.
Native plant bark material was subjected to 1.5 % alkali
treatment (5:1 ratio of waste and NaOH) and then auto-
claved for 20 min in order to remove the low molecular
weight lignin compounds. This material was then washed
with 0.001 N HCl until the pH of washing reached a
constant 6.0 ± 0.1. This fraction was then dried in an oven
at 50°C, ground to powder, and sieved at 400 lm.
Equilibrium batch experiments were conducted with
stoppered ﬂasks in a mechanical shaker incubated at
30 ± 0.2°C to evaluate the biomaterial (2 g/L) for the
removal of different metal ions separately at pH 6.0 ± 0.1.
Prior to the introduction of metal ions, ﬂasks were vigor-
ously stirred for 1.5 h to hydrate the biomaterial. After the
introduction of the metal (200 mg/L), pH was either nat-
urally buffered or adjusted with 0.1 M HNO3 to 6.0 ± 0.1.
Metal solution was allowed to equilibrate with the bio-
material for 24 h in an incubator agitated at 200 rpm. After
equilibration, samples were ﬁltered through a 0.45 lm
membrane ﬁlter and analyzed along with a control sample
for metal ions and other cations such as Ca2?
using Inductively Coupled Plasma (ICP) emission spec-
trometer (Varian Liberty-200, Palo Alto, CA). The amount
of metal adsorbed (mg) per unit mass of biomaterial (Qe)
was obtained as described by Krishnani et al. (2008a).
Two grams of biomaterial prepared from neem bark was
packed into a column with an internal diameter of 1 cm
and a column height of 15 cm. Column ends were ﬁtted
with ﬁlter disks (Millipore) of 0.45 lm pore size to retain
the material. Aqueous solution containing 20 mg/L of four
different metals (Pb, Cd, Hg, Cu) was passed through the
column containing biomaterial at a ﬂow rate of 1 mL/min
at the predetermined pH. The bed volume of the column
was 15 mL. Concentrations of metal ions and other cations
such as Ca2?
in column efﬂuents obtained at
various intervals were monitored using an ICP spectrom-
eter (Varian-Liberty 200). The column runs were carried
out to the point where the breakthrough capacity for most
of the metal ions was consumed.
X-ray photoelectron spectroscopy and Fourier transform
infrared spectra of the biomaterial after exposure to the
metal ion solution were obtained on a PHI model 5400 axis
Ultra Kratos Analytical instrument (Manchester, UK) and a
Fourier transform infrared spectrometer-FT/IR 4100 in the
range of 500–4000 cm-1
(Jasco Corp. Tokyo, Japan)
respectively at US Army Engineer Research and Devel-
opment Centre—Construction Engineering Research
Laboratory using the process as described by Krishnani
et al. (2008a). Biomaterial was ground using a ceramic
mortar and pestle in order to achieve a homogeneous and
uniform sample. Step-scanned X-ray diffraction (XRD)
patterns were collected by the Rigaku DXR-3000 com-
puter-automated diffractometer. XRD analyses were con-
ducted at 40 kV and 40 mA using Cu radiation with a
diffracted beam graphite-monochromator. The XRD pat-
tern was collected from 5° to 65° in 2h with a step size of
0.02° and a count time of 3 s per step. Qualitative XRD
analyses were performed using the JS Advanced Data
Exchange (JADE) program after background removal.
Qualitative analyses of XRD patterns were performed
using Jade software version 7.1 (MDI 2005) and the
International Center for Diffraction Data (ICDD) database
Results and Discussion
The XPS survey spectrum of neem based lignocellulosic
biomaterial loaded with metals identiﬁed two major ele-
ments (carbon and oxygen) in neem biomaterial. XRD
pattern of biomaterial prepared from neem revealed low
carbon contents, indicating the presence of inorganic pha-
ses (SiO2, Fe2O3) in neem biomaterial. Whewellite was
identiﬁed in the sample tested. Whewellite is a hydrated
calcium oxalate mineral (CaC2O4ÁH2O). Calcium ions are
electrovalently bonded with carboxylate ions, which
facilitate the ion exchange mechanism with metal ions.
The results of the maximum adsorption capacity of the
neem biomaterial at 30 ± 0.2°C and pH 6.0 ± 0.1 vis-
a`-vis maximum values adsorbed per unit mass of sorbents
from other lignocellulosic materials reported in the litera-
ture are given in Table 1. Results are either comparable or
considerably greater than those reported in the literature for
Neem biomaterial had a higher sorption capacity (mmol/
g) for copper and lead, followed by cadmium and mercury
(Table 2). Retention of metal ions onto the biomaterial
increased in the order: Hg2?
released/metal ﬁxed expressing the
percentage of ion exchange (or adsorption) indicated a
comparable quantity of ions were released from the mate-
rial, conﬁrming the ion-exchange mechanism of metal
. This indicated the bark
material contained enough Ca2?
ions to exchange with
metals ions. In the case of Hg2?
, the release of Ca2?
ions were not comparable with the maximum
quantity adsorbed onto the substrate. It could be due to
other cations involved in the ion exchange. Biomaterial did
not adsorb anionic As(III), As(V) and Cr(VI), because of
Bull Environ Contam Toxicol
their electrostatic repulsion with carboxylic functional
Hardwood bark was a better adsorbent of metals in
urban runoff compared with cypress barkpine bark nugget
(Jang et al. 2005). Hemidesmus indicus was used as bio-
material to remove Pb from aqueous streams by batch and
column experiments (Sekhar et al. 2004). Many factors
such as ionic charge, ionic radii and electrode potential are
involved in the complex reaction of metal removal capacity
of the biomass. The greater the electrode potential, the
greater the afﬁnity for biomass (Sekhar et al. 2004).
Horsfall et al. (2006) investigated the kinetics of Cd2?
adsorption onto pure and thioglycolic acid
treated cassava tuber bark wastes (CTBW), and the
monolayer sorption capacity was found to range between
5.88–26.3, 33.3–90.9 and 22.2–83.3 mg/g, respectively for
. Samecka-Cymerman et al. (2006)
investigated the suitability of bark and pine needles to
monitor metal pollution, and the study concluded that bark
was a better accumulator of Cd, Cu, Ni and an inferior
accumulator of Mn.
Experimental breakthrough curves for metal ion
adsorption onto the biomaterial at 30 ± 0.2°C are shown in
Fig. 1. Different ﬂow rates were used to achieve the
highest removal of the adsorbent which was 0.5 mL/min.
There was no leakage of Pb2?
throughout the bed
volumes with an initial concentration (Ci) of 20 mg/L. For
, there was no leakage up to 30–35 bed
volumes with an initial concentration (Ci) of 20 mg/L.
After these bed volumes, the column efﬂuent concentration
(Co) increased gradually and attained the inﬂuent concen-
tration at around 60 bed volumes.
The fast rise of efﬂuent to inﬂuent concentration with
bed volumes indicated faster kinetics adsorption. The
biomaterial exhibited greater adsorption capacity due to a
higher initial concentration and optimum pH. The column
capacity was calculated by breakthrough curves at com-
plete exhaustion, which is greater than in the batch
experiment. Large concentration gradient occurred con-
tinuously at the interface zones as it passes through the
column, which leads to high column capacity. While the
concentration gradient decreased with time in the batch
experiment. Multiple elements column ﬂow experiment
revealed the clear sorption preference for Pb2?
Similar results were obtained by Gerente et al. (2004) on
biosorption of Pb2?
on sugar beet pulp,
Table 1 Maximum adsorption capacities (mg/g) for neem biomaterial in the present study (pH 6 ± 0.1) and other lignocellulosic materials in
Material Literature Hg Cd Pb Zn Cu Ni Co Mn
Tannin adsorbent Xin-Min et al. (2001) 30–40
Adsorbent from condensed tannins Xin-Min and Zhao (2003) 57.5–114.9
Wheat bran Bulut and Baysal (2006) 69–87
Bagasse Krishnani et al. (2009) 14 3.36 24.22 3.27 7.6 2.64 2.5 0.97
Rice husk Krishnani et al. (2008a) 33.1 14.4 54 7.47 10.8 5.4 8.5 7.7
Paddy straw Krishnani et al. (2008b) 43.75 14.9 58.8 12.6 15.6 9.24 9.5 9
Black Oak Masri et al. (1974) 400 25.9 153.3 – – – – –
Hardwood bark Jang et al. (2005) 72.52 12.23 22.81 – – –
Manihotsculenta Cranz Horsfall et al. (2006) 5.88–26.3 22.2–83.3 33.3–90.9 – – –
Hemidesmum indicus Sekhar et al. (2004) – – 93.6 – – – – –
Azadirachta indica Present study 18.9 27 66.46 – 24.1 – – –
Table 2 Metal ions sorption
and corresponding ion exchange
onto the biomaterial at pH
6.0 ± 0.1 (initial metal
concentration 200 mg/L)
Metal Metal ion ﬁxed Exchangeable cations
mg/g mmol/g Ca2?
mg/g mmol/g mg/g mmol/g mmol/g %
Pb 66.46 0.32 11.4 0.284 0.766 0.0314 0.315 99
Cu 24.1 0.378 13.9 0.3468 0.65 0.0268 0.374 99
Hg 18.9 0.0942 1.39 0.0347 0.427 0.0176 0.0523 55
Cd 27.0 0.24 8.70 0.217 0.366 0.015 0.232 97
Bull Environ Contam Toxicol
and it was also reported that Ni2?
had a less competitive
Figure 2 represents the release of Ca2?
respect to bed volumes. Ca2?
ions were consistently
released from the biomaterial in a continuously decreasing
order up to 60 bed volumes. The presence of ample Ca2?
ions in neem biomaterial increased the ability to bind as
many as four metals for ion exchange and functional
groups which attract and sequester metal ions. In com-
parison to Ca2?
ions seemed to be less
dependent on Pb2?
ions, where as Mg2?
ions played a substantial role in an ion exchange of Hg2?
ions. Hanzlik et al. (2004) concluded total metal uptake
was considerably higher in a mixture than single-ion
The FTIR spectrum of biomaterial prepared from neem
bark (Fig. 3a) showed several polar groups, –OH, –NH,
–C=O, and other amino, sulfonate and phosphonate groups
which may be able to interact with metals being currently
studied. The biomaterial showed a strong band at
that refered to the NH and OH vibrational
stretches. A smaller sharp peak at 1180 cm-1
assigned to the C–N stretches of different amines. A strong
absorption band at 1030 cm-1
is characteristic of the C–O
stretch of alcohols. Two sharp peaks observed at 1690 and
are indicative of the presence of carbonyl groups
associated with amides and carboxyl groups. Peaks around
1505 and 1380 cm-1
are assigned to the N–H stretch of
primary and secondary amines. The main C–H stretch peak
of the carbon polymeric backbone is shown at 2900 cm-1
Broad bands present between 1400 and 1350 cm-1
characteristic of the asymmetric bending vibration of dif-
ferent types of aliphatic carbons and CH2 bonded to double
bonds, aromatics and carbonyls.
Pb loaded biomaterial (Fig. 3b) showed a decrease in the
intensity of the hydroxyl and free amine peaks at
. There is a considerable broadening and
shifting of the C–O peak at 1030 cm-1
indicating most of
the interaction of the bark with Pb occurred through the C–O
groups at 1030 cm-1
with minor participation of carbonyls.
The FTIR spectrum of Cu loaded biomaterial (Fig. 3c)
also showed decreased intensity of the hydroxyl and free
amine stretch bands at 3550–3250 cm-1
compared to the
native bark starting material. Carbonyl peaks for amides
and carboxyls showed broadening with bands starting at
longer wavelengths. The C–O band for alcohols in the
material showed a shift towards longer wavelengths toge-
ther with a deformation of the main band into different
smaller overlapping bands with two maximums at 1050
and 1040 cm-1
. The appearance of these additional bands
over the area of 1030 cm-1
served as evidence the alcohol
terminals together with the carbonyls of the bark material
are the main functional groups involved in the binding of
Cu. The shifting towards longer wavelengths occurring on
the Cu loaded material strongly suggested that there is a
coordination type binding between these functional groups
and the metal.
Fig. 1 Experimental
breakthrough curve for
adsorption of metal ions on
Fig. 2 Release of cations from biomaterial in column adsorption
Bull Environ Contam Toxicol
Cd spectrum (Fig. 3d) showed a shifting and broadening
band assigned to the amide carbonyl and the
appearance of two major overlapping bands at the N–H
stretches frequencies of 1505 and 1380 cm-1
. The C–O
stretch at 1030 cm-1
showed the appearance of three
overlapping absorptions shifted to longer wavelengths.
Changes in the IR absorption described suggest the binding
is primarily inﬂuenced by the presence of amines
and free hydroxyl functional groups in the bark structure.
With the exception of Hg, which remained similar to native
bark material, all the other metal loaded biomaterial
showed signiﬁcant absorption changes on the ﬁngerprint
area which suggested sulfur and phosphates were possibly
involved in the binding.
The Hg loaded biomaterial (Fig. 3e) showed a low level
of signiﬁcant changes compared to native bark material,
which is indicative of low levels of chemical interactions
between the functional groups on the bark surface and Hg.
However, the main interaction of Hg could be at the
sulfonate groups (*1050–1030 cm-1
). Peaks below
belong to the ﬁngerprint frequencies with
absorptions of the functional groups containing sulfur and
phosphates (Munagapati et al. 2010).
Dupont et al. (2006) studied adsorption isotherms of ﬁve
metal cations (Cr3?
) onto ﬁve
species of barks such as sweet chestnut, oak, Douglas ﬁr,
Norway spruce and Scots pine species and concluded Cu2?
interacted preferentially with phenolic groups present in
lignins and tannins, while Pb2?
with carboxylic acid groups
in polysaccharides. Similar conclusions have been drawn in
the present study. At a higher pH, the percentage of phe-
nolic species becomes relatively more important (Dupont
et al. 2003).
Gerente et al. (2006) observed two types of ﬁxation site
: the carboxylic sites involved in ion exchange
and those taking part in adsorption. The present
work described the retention mechanism of metal ions onto
the newly developed neem bark based biomaterial.
Fig. 3 FTIR of biomaterial and biomaterials loaded with metals. a Neem biomaterial (control sample), b Pb loaded biomaterial, c Cu loaded
biomaterial, d Cd loaded biomaterial, e Hg loaded biomaterial
Bull Environ Contam Toxicol
Whewellite (C2CaO4ÁH2O) has been identiﬁed in the bio-
material, which indicated Ca2?
ions are electrovalently
bonded with carboxylate ions facilitating the ion exchange
mechanism with metal ions. Neem bark can be used as
bioindicators, bioaccumulators and biomonitors while
determining environmental pressures. This type of struc-
tural investigation enabled an accurate prediction of the
metal bioaccumulative properties of the material, which in
turns helped in providing quantitative information on the
metal contamination in the environment around it.
Arshad M, Zafar MN, Younis S, Nadeem R (2008) The use of Neem
biomass for the biosorption of zinc from aqueous solutions.
J Hazard Mater 157(2–3):534–540
Athar M, Farooq U, Hussain B (2007) Azadirachata indicum (Neem):
an effective biosorbent for the removal of lead (II) from aqueous
solutions. Bull Environ Contam Toxicol 79(3):288–292
Bulut Y, Baysal Z (2006) Removal of Pb(II) from wastewater using
wheat bran. J Environ Manag 78:107–113
Dupont L, Bouand J, Dumonceau J, Aplincourt M (2003) Metal ions
binding onto a lignocellulosic substrate extracted from wheat
bran: a NICA–Donnan approach. J Colloid Interface Sci
Dupont MF, Gloaguen V, Guilloton M, Granet R, Krausz P (2006)
Study of the chemical interaction between barks and heavy metal
cations in the sorption process. J Environ Sci Health A
Gerente C, Reddad Z, Abdres Y, Le Cloirec P (2004) Competitive
adsorption of metals and organics onto a low cost natural
polysaccharide. Environ Technol 25:219–225
Gerente C, Du Mesnil PC, Andres Y, Thibault JF, Le Cloirec P (2006)
Removal of metal ions from aqueous solution on low cost natural
polysaccharides sorption mechanism approach. React Funct
Gloaguen V, Morvan H (1997) Removal of heavy metal ions from
aqueous solution by modiﬁed barks. J Environ Sci Health A
Hanzlik J, Jehlicka J, Sebek OO, Weishauptova Z, Machovic VV
(2004) Multi-component adsorption of Ag(I), Cd(II) and Cu(II)
by natural carbonaceous materials. Water Res 38(8):2178–2184
Horsfall M, Abia AA, Spiff AI (2006) Kinetic studies on the
adsorption of Cd2?
ions from aqueous solutions
by cassava (Manihotsculenta Cranz) tuber bark waste. Bioresour
ICDD (2002) Powder diffraction ﬁle release 2002, PDF-2: Interna-
tional Centre for Diffraction Data, Newton Square, PA
Jang A, Seo Y, Bishop PL (2005) The removal of heavy metals in
urban runoff by sorption on mulch. Environ Pollut 133(1):
Krishnani KK, Meng X, Boddu VM (2008a) Fixation of heavy metals
onto lignocellulosic sorbent prepared from paddy straw. Water
Environ Res 80:2165–2174
Krishnani KK, Ayyappan S (2006) Heavy metals remediation of
water using plant and lignocellulosic agrowastes. Rev Environ
Contam Toxicol 88:64–85
Krishnani KK, Meng X, Christodoulatos C, Boddu VM (2008b)
Biosorption mechanism of nine different heavy metals onto
biomatrix from rice husk. J Hazard Mater 153:1222–1234
Krishnani KK, Meng X, Dupont L (2009) Metal ions binding onto
lignocellulosic biosorbent. J Environ Sci Health A 44:1–12
Maharia RS, Dutta RK, Acharya R, Reddy AV (2010) Heavy metal
bioaccumulation in selected medicinal plants collected from
Khetri copper mines and comparison with those collected from
fertile soil in Haridwar, India. J Environ Sci Health B
Masri MS, Reuter FW, Friedman M (1974) Binding of metal cations
by natural substances. J Appl Polym Sci 18(3):675–681
MDI (Material’s Data Inc) (2005) Jade Version 7.1. California, USA
Munagapati VS, Yarramuthi V, Nadavala SK, Alla SR, Abburi K
(2010) Biosorption of Cu(II), Cd(II) and Pd(II) by Acacia
leucophala bark powder: kinetics, equilibrium and thermody-
namics. Chem Eng J 157:357–365
Samecka-Cymerman A, Kosior G, Kempers AJ (2006) Comparison of
the moss Pleurozium schreberi with needles and bark of Pinussyl
vestris as biomonitors of pollution by industry in Stalowa Wola
(southeast Poland). Ecotoxicol Environ Saf 65(1):108–117
Sekhar CK, Kamala CT, Chary NS, Sastry AR, Rao NT, Vairamani M
(2004) Removal of lead from aqueous solutions using an
immobilized biomaterial derived from a plant biomass.
J Hazard Mater 108:111–117
Xin-Min Z, Zhao X (2003) Mechanism of lead adsorption from
aqueous solutions using an adsorbent synthesized from natural
condensed tannins. Water Res 37:3905–3912
Xin-Min Z, Miyazaki A, Nakano Y (2001) Mechanisms of lead
removal from aqueous solutions using a novel tannin gel
adsorbent synthesized from natural condensed tannin. J Chem
Eng Jpn 34:1204–1210
Bull Environ Contam Toxicol